# Electronic Supplementary Material (ESI) for RSC Advances.
# This journal is © The Royal Society of Chemistry 2018

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_C12H18O39U6
_database_code_depnum_ccdc_archive 'CCDC 1850747'
_audit_update_record             
;
2018-06-21 deposited with the CCDC.
2018-10-08 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            'Uranium formic acid'
_chemical_melting_point          N/a
_chemical_formula_moiety         'C12 H18 O39 U6'
_chemical_formula_sum            'C12 H18 O39 U6'
_chemical_formula_weight         2214.45

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        'C 2/c'
_space_group_name_Hall           '-C 2yc'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   20.236(3)
_cell_length_b                   11.8211(16)
_cell_length_c                   16.322(2)
_cell_angle_alpha                90
_cell_angle_beta                 104.698(4)
_cell_angle_gamma                90
_cell_volume                     3776.7(9)
_cell_formula_units_Z            4
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    5124
_cell_measurement_theta_min      2.24
_cell_measurement_theta_max      27.52

_exptl_crystal_description       Rhombus
_exptl_crystal_colour            Green
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.895
_exptl_crystal_F_000             3816
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.800
_exptl_crystal_size_mid          0.500
_exptl_crystal_size_min          0.200
_exptl_absorpt_coefficient_mu    25.760
_shelx_estimated_absorpt_T_min   0.018
_shelx_estimated_absorpt_T_max   0.079
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.000
_exptl_absorpt_correction_T_max  0.006
_exptl_absorpt_process_details   SHELTXPREP

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'Turbo X-ray Source'
_diffrn_measurement_device_type  'Bruker APEX-III '
_diffrn_measurement_method       '0.5 wide w/ exposures'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            11345
_diffrn_reflns_av_unetI/netI     0.0459
_diffrn_reflns_av_R_equivalents  0.0350
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_theta_min         2.875
_diffrn_reflns_theta_max         27.536
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.967
_diffrn_measured_fraction_theta_full 0.983
_diffrn_reflns_Laue_measured_fraction_max 0.967
_diffrn_reflns_Laue_measured_fraction_full 0.983
_diffrn_reflns_point_group_measured_fraction_max 0.967
_diffrn_reflns_point_group_measured_fraction_full 0.983
_reflns_number_total             4221
_reflns_number_gt                3292
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker APEX3'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0151P)²+73.0952P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         4221
_refine_ls_number_parameters     260
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0530
_refine_ls_R_factor_gt           0.0351
_refine_ls_wR_factor_ref         0.0698
_refine_ls_wR_factor_gt          0.0652
_refine_ls_goodness_of_fit_ref   1.070
_refine_ls_restrained_S_all      1.070
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U2 U 0.43218(2) 0.33052(3) 0.08566(2) 0.01716(9) Uani 1 1 d . . . . .
U1 U 0.5000 0.56261(4) 0.2500 0.01733(11) Uani 1 2 d S T P . .
U4 U 0.5000 0.10237(4) 0.2500 0.02526(13) Uani 1 2 d S T P . .
U3 U 0.62070(2) 0.33670(3) 0.20693(2) 0.02056(9) Uani 1 1 d . . . . .
O1 O 0.5182(4) 0.6726(5) 0.0337(4) 0.0335(17) Uani 1 1 d . . . . .
O2 O 0.4056(4) 0.1517(5) 0.0142(4) 0.0295(16) Uani 1 1 d . . . . .
O3 O 0.3965(3) 0.2053(5) 0.1836(4) 0.0230(14) Uani 1 1 d . . . . .
H3B H 0.3570 0.1577 0.1582 0.028 Uiso 1 1 calc R U . . .
O4 O 0.5275(3) 0.4622(5) 0.1316(3) 0.0178(13) Uani 1 1 d . . . . .
H4B H 0.5377 0.5099 0.0872 0.021 Uiso 1 1 calc R U . . .
O5 O 0.6035(4) 0.5083(6) 0.0041(4) 0.0342(16) Uani 1 1 d . . . . .
O6 O 0.4231(3) 0.4293(5) 0.1993(4) 0.0191(13) Uani 1 1 d . . . . .
O7 O 0.6048(4) 0.6539(6) 0.2391(5) 0.0389(18) Uani 1 1 d . . . . .
O8 O 0.3089(4) 0.3421(6) 0.0549(4) 0.0333(16) Uani 1 1 d . . . . .
O9 O 0.6728(4) 0.5232(6) 0.2039(4) 0.0331(16) Uani 1 1 d . . . . .
O10 O 0.4692(4) 0.7028(6) 0.1386(4) 0.0386(19) Uani 1 1 d . . . . .
O11 O 0.6414(4) 0.3481(6) 0.0685(5) 0.045(2) Uani 1 1 d . . . . .
O12 O 0.2788(3) 0.3408(7) 0.1774(4) 0.0370(18) Uani 1 1 d . . . . .
O13 O 0.5216(3) 0.2430(5) 0.1631(4) 0.0208(14) Uani 1 1 d . . . . .
O14 O 0.4523(4) 0.0197(5) 0.1092(4) 0.0391(19) Uani 1 1 d . . . . .
O15 O 0.6665(4) 0.1568(7) 0.1792(5) 0.047(2) Uani 1 1 d . . . . .
O16 O 0.5973(5) 0.0217(6) 0.2043(5) 0.050(2) Uani 1 1 d . . . . .
O17 O 0.5000 -0.1057(9) 0.2500 0.093(6) Uani 1 2 d S T P . .
H17A H 0.4890 -0.1451 0.2941 0.111 Uiso 0.5 1 calc R U P . .
H17B H 0.5110 -0.1451 0.2059 0.111 Uiso 0.5 1 calc R U P . .
C1 C 0.6573(6) 0.6202(10) 0.2201(7) 0.043(3) Uani 1 1 d . . . . .
H1A H 0.6893 0.6758 0.2179 0.052 Uiso 1 1 calc R U . . .
C2 C 0.6377(6) 0.4203(9) 0.0115(7) 0.039(3) Uani 1 1 d . . . . .
H2A H 0.6625 0.4069 -0.0283 0.047 Uiso 1 1 calc R U . . .
C3 C 0.2653(5) 0.3428(9) 0.0974(6) 0.033(2) Uani 1 1 d . . . . .
H3A H 0.2195 0.3450 0.0678 0.039 Uiso 1 1 calc R U . . .
C4 C 0.6497(8) 0.0564(12) 0.1866(7) 0.052(4) Uani 1 1 d . . . . .
H4A H 0.6801 0.0014 0.1780 0.062 Uiso 1 1 calc R U . . .
C5 C 0.4188(6) 0.0521(8) 0.0380(6) 0.034(3) Uani 1 1 d . . . . .
H5A H 0.4019 -0.0041 -0.0016 0.041 Uiso 1 1 calc R U . . .
C6 C 0.4910(7) 0.7341(9) 0.0766(7) 0.044(3) Uani 1 1 d . . . . .
H6A H 0.4862 0.8102 0.0619 0.053 Uiso 1 1 calc R U . . .
O1W O 0.830(2) 0.341(4) 0.153(3) 0.087(12) Uiso 0.3 1 d . . P . .
O2W O 0.7566(17) 0.180(3) 0.092(2) 0.086(9) Uiso 0.35 1 d . . P . .
O1WA O 0.7576(14) 0.344(2) 0.1751(18) 0.084(8) Uiso 0.4 1 d . . P . .
O3W O 0.2846(4) 0.0703(7) 0.1116(6) 0.057(2) Uiso 1 1 d . . . . .
O1WB O 0.826(2) 0.328(3) 0.100(3) 0.074(10) Uiso 0.3 1 d . . P . .
O2WA O 0.792(2) 0.297(3) 0.125(3) 0.078(11) Uiso 0.3 1 d . . P . .
O2WB O 0.7273(18) 0.133(3) 0.041(2) 0.091(10) Uiso 0.35 1 d . . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U2 O13 2.187(6) . ?
U2 O6 2.238(5) . ?
U2 O5 2.399(7) 5_665 ?
U2 O1 2.407(6) 5_665 ?
U2 O2 2.408(6) . ?
U2 O3 2.419(6) . ?
U2 O8 2.420(7) . ?
U2 O4 2.444(6) . ?
U2 U3 3.8011(6) 2_655 ?
U2 U4 3.8058(6) . ?
U2 U3 3.8270(7) . ?
U2 U1 3.8390(6) . ?
U1 O6 2.222(6) . ?
U1 O6 2.222(6) 2_655 ?
U1 O10 2.421(6) 2_655 ?
U1 O10 2.422(6) . ?
U1 O7 2.426(7) 2_655 ?
U1 O7 2.426(7) . ?
U1 O4 2.449(5) 2_655 ?
U1 O4 2.449(5) . ?
U1 U3 3.8030(6) 2_655 ?
U1 U3 3.8031(6) . ?
U1 U2 3.8389(6) 2_655 ?
U4 O13 2.297(6) 2_655 ?
U4 O13 2.297(6) . ?
U4 O3 2.427(6) . ?
U4 O3 2.427(6) 2_655 ?
U4 O14 2.458(7) 2_655 ?
U4 O14 2.458(7) . ?
U4 O16 2.468(9) 2_655 ?
U4 O16 2.468(9) . ?
U4 O17 2.460(11) . ?
U4 U2 3.8057(6) 2_655 ?
U4 U3 3.8736(6) 2_655 ?
U3 O6 2.240(5) 2_655 ?
U3 O13 2.244(6) . ?
U3 O12 2.400(7) 2_655 ?
U3 O11 2.403(7) . ?
U3 O15 2.408(7) . ?
U3 O9 2.449(7) . ?
U3 O3 2.458(6) 2_655 ?
U3 O4 2.468(6) . ?
U3 O1WA 2.95(3) . ?
U3 U2 3.8012(6) 2_655 ?
O1 C6 1.231(11) . ?
O1 U2 2.407(6) 5_665 ?
O2 C5 1.248(11) . ?
O3 U3 2.458(6) 2_655 ?
O5 C2 1.238(12) . ?
O5 U2 2.399(7) 5_665 ?
O6 U3 2.240(5) 2_655 ?
O7 C1 1.245(13) . ?
O8 C3 1.254(12) . ?
O9 C1 1.235(13) . ?
O10 C6 1.258(12) . ?
O11 C2 1.251(12) . ?
O12 C3 1.264(12) . ?
O12 U3 2.399(7) 2_655 ?
O14 C5 1.247(12) . ?
O15 C4 1.249(16) . ?
O16 C4 1.237(16) . ?
O1W O1WB 0.85(5) . ?
O1W O2WA 0.95(5) . ?
O1W O1WA 1.61(5) . ?
O2W O2WB 1.06(4) . ?
O2W O2WA 1.58(5) . ?
O1WA O2WA 1.33(4) . ?
O1WB O2WA 0.95(5) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O13 U2 O6 89.9(2) . . ?
O13 U2 O5 143.6(2) . 5_665 ?
O6 U2 O5 90.9(2) . 5_665 ?
O13 U2 O1 90.4(2) . 5_665 ?
O6 U2 O1 144.8(2) . 5_665 ?
O5 U2 O1 69.0(2) 5_665 5_665 ?
O13 U2 O2 85.1(2) . . ?
O6 U2 O2 143.5(2) . . ?
O5 U2 O2 113.9(2) 5_665 . ?
O1 U2 O2 71.5(2) 5_665 . ?
O13 U2 O3 70.7(2) . . ?
O6 U2 O3 70.8(2) . . ?
O5 U2 O3 142.7(2) 5_665 . ?
O1 U2 O3 141.3(2) 5_665 . ?
O2 U2 O3 73.5(2) . . ?
O13 U2 O8 143.6(2) . . ?
O6 U2 O8 81.1(2) . . ?
O5 U2 O8 72.2(2) 5_665 . ?
O1 U2 O8 116.9(2) 5_665 . ?
O2 U2 O8 81.8(2) . . ?
O3 U2 O8 73.0(2) . . ?
O13 U2 O4 69.6(2) . . ?
O6 U2 O4 68.75(19) . . ?
O5 U2 O4 76.9(2) 5_665 . ?
O1 U2 O4 78.4(2) 5_665 . ?
O2 U2 O4 140.3(2) . . ?
O3 U2 O4 122.11(19) . . ?
O8 U2 O4 136.0(2) . . ?
O13 U2 U3 82.68(15) . 2_655 ?
O6 U2 U3 31.93(14) . 2_655 ?
O5 U2 U3 114.79(16) 5_665 2_655 ?
O1 U2 U3 172.02(17) 5_665 2_655 ?
O2 U2 U3 111.70(15) . 2_655 ?
O3 U2 U3 39.17(14) . 2_655 ?
O8 U2 U3 71.07(15) . 2_655 ?
O4 U2 U3 95.35(13) . 2_655 ?
O13 U2 U4 32.82(16) . . ?
O6 U2 U4 82.92(15) . . ?
O5 U2 U4 172.54(17) 5_665 . ?
O1 U2 U4 114.18(16) 5_665 . ?
O2 U2 U4 73.50(15) . . ?
O3 U2 U4 38.32(15) . . ?
O8 U2 U4 110.78(16) . . ?
O4 U2 U4 96.87(13) . . ?
U3 U2 U4 61.224(10) 2_655 . ?
O13 U2 U3 30.69(16) . . ?
O6 U2 U3 80.91(16) . . ?
O5 U2 U3 113.98(17) 5_665 . ?
O1 U2 U3 81.57(17) 5_665 . ?
O2 U2 U3 109.78(17) . . ?
O3 U2 U3 95.47(15) . . ?
O8 U2 U3 161.08(15) . . ?
O4 U2 U3 39.05(13) . . ?
U3 U2 U3 90.457(13) 2_655 . ?
U4 U2 U3 60.994(8) . . ?
O13 U2 U1 80.65(15) . . ?
O6 U2 U1 30.46(14) . . ?
O5 U2 U1 81.83(17) 5_665 . ?
O1 U2 U1 115.34(16) 5_665 . ?
O2 U2 U1 164.18(15) . . ?
O3 U2 U1 95.12(14) . . ?
O8 U2 U1 105.75(16) . . ?
O4 U2 U1 38.37(13) . . ?
U3 U2 U1 59.703(9) 2_655 . ?
U4 U2 U1 90.742(14) . . ?
U3 U2 U1 59.484(8) . . ?
O6 U1 O6 89.7(3) . 2_655 ?
O6 U1 O10 141.9(2) . 2_655 ?
O6 U1 O10 100.5(2) 2_655 2_655 ?
O6 U1 O10 100.6(2) . . ?
O6 U1 O10 141.9(2) 2_655 . ?
O10 U1 O10 93.6(4) 2_655 . ?
O6 U1 O7 78.5(2) . 2_655 ?
O6 U1 O7 146.2(2) 2_655 2_655 ?
O10 U1 O7 72.8(3) 2_655 2_655 ?
O10 U1 O7 71.8(2) . 2_655 ?
O6 U1 O7 146.2(2) . . ?
O6 U1 O7 78.5(2) 2_655 . ?
O10 U1 O7 71.8(2) 2_655 . ?
O10 U1 O7 72.8(3) . . ?
O7 U1 O7 127.2(3) 2_655 . ?
O6 U1 O4 70.88(19) . 2_655 ?
O6 U1 O4 68.9(2) 2_655 2_655 ?
O10 U1 O4 78.8(2) 2_655 2_655 ?
O10 U1 O4 149.0(2) . 2_655 ?
O7 U1 O4 77.3(2) 2_655 2_655 ?
O7 U1 O4 130.6(2) . 2_655 ?
O6 U1 O4 68.9(2) . . ?
O6 U1 O4 70.88(19) 2_655 . ?
O10 U1 O4 149.0(2) 2_655 . ?
O10 U1 O4 78.8(2) . . ?
O7 U1 O4 130.6(2) 2_655 . ?
O7 U1 O4 77.3(2) . . ?
O4 U1 O4 122.0(3) 2_655 . ?
O6 U1 U3 31.68(14) . 2_655 ?
O6 U1 U3 81.66(15) 2_655 2_655 ?
O10 U1 U3 113.36(16) 2_655 2_655 ?
O10 U1 U3 124.37(19) . 2_655 ?
O7 U1 U3 71.59(17) 2_655 2_655 ?
O7 U1 U3 160.10(18) . 2_655 ?
O4 U1 U3 39.52(13) 2_655 2_655 ?
O4 U1 U3 95.21(13) . 2_655 ?
O6 U1 U3 81.66(15) . . ?
O6 U1 U3 31.68(14) 2_655 . ?
O10 U1 U3 124.37(19) 2_655 . ?
O10 U1 U3 113.36(16) . . ?
O7 U1 U3 160.10(18) 2_655 . ?
O7 U1 U3 71.59(17) . . ?
O4 U1 U3 95.21(13) 2_655 . ?
O4 U1 U3 39.52(13) . . ?
U3 U1 U3 90.792(17) 2_655 . ?
O6 U1 U2 81.14(15) . 2_655 ?
O6 U1 U2 30.71(14) 2_655 2_655 ?
O10 U1 U2 89.21(18) 2_655 2_655 ?
O10 U1 U2 172.66(16) . 2_655 ?
O7 U1 U2 115.52(17) 2_655 2_655 ?
O7 U1 U2 101.82(18) . 2_655 ?
O4 U1 U2 38.28(14) 2_655 2_655 ?
O4 U1 U2 95.30(13) . 2_655 ?
U3 U1 U2 60.100(12) 2_655 2_655 ?
U3 U1 U2 59.654(11) . 2_655 ?
O6 U1 U2 30.71(14) . . ?
O6 U1 U2 81.14(15) 2_655 . ?
O10 U1 U2 172.66(16) 2_655 . ?
O10 U1 U2 89.21(18) . . ?
O7 U1 U2 101.82(18) 2_655 . ?
O7 U1 U2 115.52(17) . . ?
O4 U1 U2 95.30(13) 2_655 . ?
O4 U1 U2 38.28(14) . . ?
U3 U1 U2 59.654(11) 2_655 . ?
U3 U1 U2 60.101(12) . . ?
U2 U1 U2 88.766(17) 2_655 . ?
O13 U4 O13 87.3(3) 2_655 . ?
O13 U4 O3 68.6(2) 2_655 . ?
O13 U4 O3 68.9(2) . . ?
O13 U4 O3 68.9(2) 2_655 2_655 ?
O13 U4 O3 68.6(2) . 2_655 ?
O3 U4 O3 119.8(3) . 2_655 ?
O13 U4 O14 78.6(2) 2_655 2_655 ?
O13 U4 O14 140.7(2) . 2_655 ?
O3 U4 O14 135.0(2) . 2_655 ?
O3 U4 O14 72.1(2) 2_655 2_655 ?
O13 U4 O14 140.7(2) 2_655 . ?
O13 U4 O14 78.6(2) . . ?
O3 U4 O14 72.1(2) . . ?
O3 U4 O14 135.0(2) 2_655 . ?
O14 U4 O14 133.2(3) 2_655 . ?
O13 U4 O16 78.6(2) 2_655 2_655 ?
O13 U4 O16 139.2(2) . 2_655 ?
O3 U4 O16 70.4(2) . 2_655 ?
O3 U4 O16 136.3(2) 2_655 2_655 ?
O14 U4 O16 73.6(3) 2_655 2_655 ?
O14 U4 O16 88.6(3) . 2_655 ?
O13 U4 O16 139.2(2) 2_655 . ?
O13 U4 O16 78.6(2) . . ?
O3 U4 O16 136.3(2) . . ?
O3 U4 O16 70.4(2) 2_655 . ?
O14 U4 O16 88.6(3) 2_655 . ?
O14 U4 O16 73.6(3) . . ?
O16 U4 O16 134.5(4) 2_655 . ?
O13 U4 O17 136.34(14) 2_655 . ?
O13 U4 O17 136.34(14) . . ?
O3 U4 O17 120.09(14) . . ?
O3 U4 O17 120.09(14) 2_655 . ?
O14 U4 O17 66.58(15) 2_655 . ?
O14 U4 O17 66.58(15) . . ?
O16 U4 O17 67.3(2) 2_655 . ?
O16 U4 O17 67.3(2) . . ?
O13 U4 U2 31.06(15) 2_655 2_655 ?
O13 U4 U2 80.28(14) . 2_655 ?
O3 U4 U2 94.33(14) . 2_655 ?
O3 U4 U2 38.18(14) 2_655 2_655 ?
O14 U4 U2 68.71(15) 2_655 2_655 ?
O14 U4 U2 157.89(15) . 2_655 ?
O16 U4 U2 103.5(2) 2_655 2_655 ?
O16 U4 U2 108.32(19) . 2_655 ?
O17 U4 U2 135.126(9) . 2_655 ?
O13 U4 U2 80.28(14) 2_655 . ?
O13 U4 U2 31.06(15) . . ?
O3 U4 U2 38.18(14) . . ?
O3 U4 U2 94.33(14) 2_655 . ?
O14 U4 U2 157.89(15) 2_655 . ?
O14 U4 U2 68.71(15) . . ?
O16 U4 U2 108.32(19) 2_655 . ?
O16 U4 U2 103.5(2) . . ?
O17 U4 U2 135.125(9) . . ?
U2 U4 U2 89.749(17) 2_655 . ?
O13 U4 U3 31.05(15) 2_655 2_655 ?
O13 U4 U3 79.74(14) . 2_655 ?
O3 U4 U3 37.82(14) . 2_655 ?
O3 U4 U3 94.18(14) 2_655 2_655 ?
O14 U4 U3 103.35(17) 2_655 2_655 ?
O14 U4 U3 109.73(17) . 2_655 ?
O16 U4 U3 68.5(2) 2_655 2_655 ?
O16 U4 U3 156.9(2) . 2_655 ?
O17 U4 U3 135.653(9) . 2_655 ?
U2 U4 U3 59.772(11) 2_655 2_655 ?
U2 U4 U3 59.329(11) . 2_655 ?
O6 U3 O13 89.0(2) 2_655 . ?
O6 U3 O12 81.7(2) 2_655 2_655 ?
O13 U3 O12 140.5(2) . 2_655 ?
O6 U3 O11 144.0(2) 2_655 . ?
O13 U3 O11 94.8(3) . . ?
O12 U3 O11 115.1(3) 2_655 . ?
O6 U3 O15 142.9(2) 2_655 . ?
O13 U3 O15 81.9(3) . . ?
O12 U3 O15 82.9(3) 2_655 . ?
O11 U3 O15 72.9(2) . . ?
O6 U3 O9 79.7(2) 2_655 . ?
O13 U3 O9 142.4(2) . . ?
O12 U3 O9 73.4(2) 2_655 . ?
O11 U3 O9 75.6(2) . . ?
O15 U3 O9 127.1(3) . . ?
O6 U3 O3 70.0(2) 2_655 2_655 ?
O13 U3 O3 68.9(2) . 2_655 ?
O12 U3 O3 71.9(2) 2_655 2_655 ?
O11 U3 O3 144.0(2) . 2_655 ?
O15 U3 O3 73.2(2) . 2_655 ?
O9 U3 O3 136.4(2) . 2_655 ?
O6 U3 O4 70.24(19) 2_655 . ?
O13 U3 O4 68.3(2) . . ?
O12 U3 O4 140.2(2) 2_655 . ?
O11 U3 O4 77.9(2) . . ?
O15 U3 O4 136.0(2) . . ?
O9 U3 O4 74.2(2) . . ?
O3 U3 O4 120.7(2) 2_655 . ?
O6 U3 O1WA 131.2(6) 2_655 . ?
O13 U3 O1WA 139.7(6) . . ?
O12 U3 O1WA 59.4(6) 2_655 . ?
O11 U3 O1WA 55.8(6) . . ?
O15 U3 O1WA 64.5(6) . . ?
O9 U3 O1WA 62.6(6) . . ?
O3 U3 O1WA 117.4(6) 2_655 . ?
O4 U3 O1WA 121.9(5) . . ?
O6 U3 U2 31.90(14) 2_655 2_655 ?
O13 U3 U2 80.98(15) . 2_655 ?
O12 U3 U2 70.94(15) 2_655 2_655 ?
O11 U3 U2 173.55(19) . 2_655 ?
O15 U3 U2 111.05(18) . 2_655 ?
O9 U3 U2 104.80(16) . 2_655 ?
O3 U3 U2 38.43(13) 2_655 2_655 ?
O4 U3 U2 95.91(13) . 2_655 ?
O1WA U3 U2 130.3(6) . 2_655 ?
O6 U3 U1 31.38(15) 2_655 . ?
O13 U3 U1 80.88(15) . . ?
O12 U3 U1 107.24(18) 2_655 . ?
O11 U3 U1 114.05(16) . . ?
O15 U3 U1 161.9(2) . . ?
O9 U3 U1 70.85(16) . . ?
O3 U3 U1 95.35(14) 2_655 . ?
O4 U3 U1 39.16(12) . . ?
O1WA U3 U1 133.5(5) . . ?
U2 U3 U1 60.642(8) 2_655 . ?
O6 U3 U2 81.22(16) 2_655 . ?
O13 U3 U2 29.83(14) . . ?
O12 U3 U2 160.43(15) 2_655 . ?
O11 U3 U2 84.4(2) . . ?
O15 U3 U2 105.4(2) . . ?
O9 U3 U2 112.61(17) . . ?
O3 U3 U2 93.29(15) 2_655 . ?
O4 U3 U2 38.60(13) . . ?
O1WA U3 U2 140.2(6) . . ?
U2 U3 U2 89.499(13) 2_655 . ?
U1 U3 U2 60.415(10) . . ?
C6 O1 U2 143.9(7) . 5_665 ?
C5 O2 U2 132.3(6) . . ?
U2 O3 U4 103.5(2) . . ?
U2 O3 U3 102.4(2) . 2_655 ?
U4 O3 U3 104.9(2) . 2_655 ?
U2 O4 U1 103.4(2) . . ?
U2 O4 U3 102.4(2) . . ?
U1 O4 U3 101.3(2) . . ?
C2 O5 U2 143.2(7) . 5_665 ?
U1 O6 U2 118.8(2) . . ?
U1 O6 U3 116.9(2) . 2_655 ?
U2 O6 U3 116.2(2) . 2_655 ?
C1 O7 U1 133.9(7) . . ?
C3 O8 U2 136.0(6) . . ?
C1 O9 U3 134.2(7) . . ?
C6 O10 U1 136.8(7) . . ?
C2 O11 U3 138.2(7) . . ?
C3 O12 U3 137.0(6) . 2_655 ?
U2 O13 U3 119.5(3) . . ?
U2 O13 U4 116.1(3) . . ?
U3 O13 U4 117.1(2) . . ?
C5 O14 U4 137.8(6) . . ?
C4 O15 U3 133.9(8) . . ?
C4 O16 U4 137.7(8) . . ?
O9 C1 O7 129.0(11) . . ?
O5 C2 O11 125.0(10) . . ?
O8 C3 O12 125.0(9) . . ?
O16 C4 O15 127.5(11) . . ?
O14 C5 O2 127.1(9) . . ?
O1 C6 O10 125.6(10) . . ?
O1WB O1W O2WA 64(4) . . ?
O1WB O1W O1WA 112(5) . . ?
O2WA O1W O1WA 56(4) . . ?
O2WB O2W O2WA 148(4) . . ?
O2WA O1WA O1W 36(2) . . ?
O2WA O1WA U3 140(2) . . ?
O1W O1WA U3 176(2) . . ?
O1W O1WB O2WA 63(4) . . ?
O1W O2WA O1WB 53(4) . . ?
O1W O2WA O1WA 88(5) . . ?
O1WB O2WA O1WA 131(5) . . ?
O1W O2WA O2W 153(5) . . ?
O1WB O2WA O2W 120(5) . . ?
O1WA O2WA O2W 108(3) . . ?

_refine_diff_density_max         1.555
_refine_diff_density_min         -1.355
_refine_diff_density_rms         0.258

_shelxl_version_number           2014-3



####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_SAVE
_database_code_depnum_ccdc_archive 'CCDC 1850748'
_audit_update_record             
;
2018-06-21 deposited with the CCDC.
2018-10-08 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            'Uranium formic acid'
_chemical_melting_point          n/a
_chemical_formula_moiety         'C13 O38 U6'
_chemical_formula_sum            'C13 O38 U6'
_chemical_formula_weight         2192.31

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.5396(5)
_cell_length_b                   11.7744(8)
_cell_length_c                   16.2574(8)
_cell_angle_alpha                77.994(3)
_cell_angle_beta                 77.951(2)
_cell_angle_gamma                60.742(2)
_cell_volume                     1870.07(18)
_cell_formula_units_Z            2
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    10777
_cell_measurement_theta_min      2.173
_cell_measurement_theta_max      30.157

_exptl_crystal_description       Rhombus
_exptl_crystal_colour            green
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.893
_exptl_crystal_F_000             1868
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.750
_exptl_crystal_size_mid          0.460
_exptl_crystal_size_min          0.230
_exptl_absorpt_coefficient_mu    26.008
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.000
_exptl_absorpt_correction_T_max  0.003
_exptl_absorpt_process_details   sheltxprep

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'Turbo X-ray Source'
_diffrn_measurement_device_type  'Bruker APEX-III '
_diffrn_measurement_method       '0.5 wide w/ exposures'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            10777
_diffrn_reflns_av_unetI/netI     0.0676
_diffrn_reflns_av_R_equivalents  ?
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_theta_min         2.173
_diffrn_reflns_theta_max         30.157
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.974
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.974
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.974
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             10777
_reflns_number_gt                7370
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker APEX3'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 Refined as a 2-component twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0471P)²+40.0360P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         10777
_refine_ls_number_parameters     515
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0816
_refine_ls_R_factor_gt           0.0438
_refine_ls_wR_factor_ref         0.1046
_refine_ls_wR_factor_gt          0.0901
_refine_ls_goodness_of_fit_ref   0.901
_refine_ls_restrained_S_all      0.901
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U6 U 0.43408(4) 0.55722(4) 0.75190(2) 0.01413(9) Uani 1 1 d . . . . .
U5 U 0.73816(4) 0.39806(4) 0.58672(2) 0.01370(9) Uani 1 1 d . . . . .
U4 U 0.60554(4) 0.26249(4) 0.91423(2) 0.01427(9) Uani 1 1 d . . . . .
U3 U 0.78314(4) 0.46229(4) 0.79376(2) 0.01570(9) Uani 1 1 d . . . . .
U2 U 0.54829(4) 0.21038(4) 0.70588(2) 0.01605(9) Uani 1 1 d . . . . .
U1 U 0.90705(4) 0.10792(4) 0.75138(2) 0.01741(10) Uani 1 1 d . . . . .
O33 O 0.6460(7) 0.5067(7) 0.7006(5) 0.0180(16) Uani 1 1 d . . . . .
O32 O 0.4967(7) 0.3474(7) 0.8002(4) 0.0130(14) Uani 1 1 d . . . . .
O31 O 0.7842(7) 0.2686(7) 0.8370(4) 0.0146(15) Uani 1 1 d . . . . .
O30 O 0.5097(7) 0.4301(7) 0.6316(4) 0.0150(15) Uani 1 1 d . . . . .
O29 O 0.6964(8) 0.3477(8) 0.4633(5) 0.0264(19) Uani 1 1 d . . . . .
O28 O 0.5646(7) 0.4900(7) 0.8693(4) 0.0171(16) Uani 1 1 d . . . . .
O27 O 0.7411(7) 0.2208(7) 0.6635(5) 0.0179(16) Uani 1 1 d . . . . .
O26 O 0.6075(8) 0.5942(8) 0.4985(5) 0.0260(19) Uani 1 1 d . . . . .
O25 O 0.8476(9) 0.5367(8) 0.5552(5) 0.0276(19) Uani 1 1 d . . . . .
O24 O 0.6439(9) 0.6980(8) 0.7981(5) 0.0288(19) Uani 1 1 d . . . . .
O23 O 0.2403(8) 0.5397(9) 0.7378(6) 0.033(2) Uani 1 1 d . . . . .
O22 O 0.9022(8) 0.3137(8) 0.6834(5) 0.0199(16) Uani 1 1 d . . . . .
O21 O 0.6990(8) 0.1013(7) 0.8156(5) 0.0186(16) Uani 1 1 d . . . . .
O20 O 0.4411(9) 0.7541(8) 0.7669(6) 0.030(2) Uani 1 1 d . . . . .
O19 O 0.3136(9) 0.7324(8) 0.6447(5) 0.029(2) Uani 1 1 d . . . . .
O18 O 0.6600(9) 0.3157(8) 1.0322(5) 0.029(2) Uani 1 1 d . . . . .
O17 O 1.1303(9) -0.0908(9) 0.7545(6) 0.038(2) Uani 1 1 d . . . . .
O16 O 0.9000(11) -0.0768(9) 0.7063(6) 0.041(2) Uani 1 1 d . . . . .
O15 O 1.0813(9) 0.1352(9) 0.7994(6) 0.037(2) Uani 1 1 d . . . . .
O14 O 0.9490(8) 0.2486(8) 0.5160(5) 0.0246(18) Uani 1 1 d . . . . .
O13 O 0.9396(8) -0.0220(9) 0.8936(5) 0.031(2) Uani 1 1 d . . . . .
O12 O 0.8761(9) 0.5697(9) 0.6786(5) 0.031(2) Uani 1 1 d . . . . .
O11 O 0.7582(8) 0.0607(8) 0.9866(5) 0.0269(19) Uani 1 1 d . . . . .
O10 O 0.3079(8) 0.3427(8) 0.7010(5) 0.0256(18) Uani 1 1 d . . . . .
O9 O 0.4727(8) 0.1478(8) 0.9464(5) 0.0253(18) Uani 1 1 d . . . . .
O8 O 0.6992(10) -0.0158(9) 0.6743(6) 0.035(2) Uani 1 1 d . . . . .
O7 O 0.4062(9) 0.3864(9) 1.0028(6) 0.032(2) Uani 1 1 d . . . . .
O6 O 0.4443(9) 0.1151(10) 0.8234(6) 0.034(2) Uani 1 1 d . . . . .
O5 O 0.2644(9) 0.6536(9) 0.8650(5) 0.031(2) Uani 1 1 d . . . . .
O4 O 0.4710(10) 0.7898(9) 0.4396(6) 0.039(2) Uani 1 1 d . . . . .
O3 O 1.0128(9) 0.3378(10) 0.8209(6) 0.034(2) Uani 1 1 d . . . . .
O2 O 0.2061(8) 0.4961(10) 1.0699(5) 0.036(2) Uani 1 1 d . . . . .
O1 O 1.0392(10) 0.0729(9) 0.6101(5) 0.034(2) Uani 1 1 d . . . . .
C7 C 0.5227(14) 0.7787(12) 0.7886(7) 0.026(3) Uani 1 1 d . . . . .
C6 C 0.5435(13) 0.7148(12) 0.4959(8) 0.028(3) Uani 1 1 d . . . . .
C5 C 0.2200(12) 0.4563(13) 0.7169(8) 0.026(3) Uani 1 1 d . . . . .
C4 C 0.4304(14) 0.1034(14) 0.9035(9) 0.035(3) Uani 1 1 d . . . . .
C3 C 0.8901(14) 0.5816(13) 0.5997(9) 0.031(3) Uani 1 1 d . . . . .
C2 C 0.2833(13) 0.4277(15) 1.0143(8) 0.035(3) Uani 1 1 d . . . . .
C1 C 0.8751(13) -0.0245(12) 0.9638(8) 0.029(3) Uani 1 1 d . . . . .
C12 C 0.2607(15) 0.7395(12) 0.5830(8) 0.032(3) Uani 1 1 d . . . . .
C11 C 1.0387(13) 0.1369(13) 0.5397(8) 0.032(3) Uani 1 1 d . . . . .
C10 C 1.0998(13) 0.2199(13) 0.8148(8) 0.029(3) Uani 1 1 d . . . . .
C9 C 0.8179(16) -0.1008(13) 0.6869(9) 0.038(3) Uani 1 1 d . . . . .
C8 C 0.7501(14) 0.2897(15) 1.0727(9) 0.040(4) Uani 1 1 d . . . . .
OW2 O 1.1475(9) 0.2948(10) 0.6056(6) 0.037(2) Uani 1 1 d . . . . .
OW1 O 0.7264(13) -0.1442(10) 0.8827(8) 0.058(3) Uani 1 1 d . . . . .
OW3 O 0.991(2) -0.367(3) 0.8747(18) 0.183(11) Uani 1 1 d . . . . .
O35 O 0.4080(16) 0.0835(14) 0.6709(9) 0.078(4) Uani 1 1 d . . . . .
O34 O 0.5654(19) -0.0857(16) 0.6019(12) 0.105(6) Uani 1 1 d . . . . .
C13 C 0.430(3) 0.0004(19) 0.6243(15) 0.080(7) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U6 O32 2.220(7) . ?
U6 O33 2.227(7) . ?
U6 O5 2.387(9) . ?
U6 O23 2.404(8) . ?
U6 O20 2.422(8) . ?
U6 O19 2.436(8) . ?
U6 O28 2.438(7) . ?
U6 O30 2.460(7) . ?
U6 U3 3.7900(6) . ?
U6 U4 3.8185(6) . ?
U6 U2 3.8174(6) . ?
U6 U5 3.8428(6) . ?
U5 O27 2.187(7) . ?
U5 O33 2.242(7) . ?
U5 O26 2.405(8) . ?
U5 O29 2.406(7) . ?
U5 O14 2.414(8) . ?
U5 O22 2.408(7) . ?
U5 O25 2.433(8) . ?
U5 O30 2.442(7) . ?
U5 U3 3.7871(6) . ?
U5 U1 3.8078(6) . ?
U5 U2 3.8230(6) . ?
U4 O31 2.204(7) . ?
U4 O32 2.233(7) . ?
U4 O7 2.388(8) . ?
U4 O11 2.397(8) . ?
U4 O9 2.416(8) . ?
U4 O21 2.425(8) . ?
U4 O18 2.419(8) . ?
U4 O28 2.455(8) . ?
U4 U1 3.7943(6) . ?
U4 U2 3.8055(6) . ?
U4 U3 3.8328(6) . ?
U3 O33 2.222(7) . ?
U3 O31 2.238(7) . ?
U3 O3 2.406(9) . ?
U3 O2 2.407(8) 2_667 ?
U3 O12 2.399(8) . ?
U3 O24 2.442(9) . ?
U3 O28 2.458(7) . ?
U3 O22 2.468(8) . ?
U3 U1 3.8576(6) . ?
U2 O27 2.243(8) . ?
U2 O32 2.239(7) . ?
U2 O6 2.411(9) . ?
U2 O4 2.421(9) 2_666 ?
U2 O10 2.438(8) . ?
U2 O21 2.452(7) . ?
U2 O8 2.460(9) . ?
U2 O30 2.479(7) . ?
U2 O35 2.877(14) . ?
U1 O31 2.275(7) . ?
U1 O27 2.310(7) . ?
U1 O22 2.424(8) . ?
U1 O21 2.442(8) . ?
U1 O1 2.468(9) . ?
U1 O15 2.479(10) . ?
U1 O13 2.481(8) . ?
U1 O16 2.477(10) . ?
U1 O17 2.496(8) . ?
O29 C12 1.239(14) 2_666 ?
O26 C6 1.236(14) . ?
O25 C3 1.267(15) . ?
O24 C7 1.270(15) . ?
O23 C5 1.238(15) . ?
O20 C7 1.242(15) . ?
O19 C12 1.248(14) . ?
O18 C8 1.225(15) . ?
O16 C9 1.225(18) . ?
O15 C10 1.199(16) . ?
O14 C11 1.255(15) . ?
O13 C1 1.230(14) . ?
O12 C3 1.246(15) . ?
O11 C1 1.260(15) . ?
O10 C5 1.263(15) . ?
O9 C4 1.242(16) . ?
O8 C9 1.269(17) . ?
O7 C2 1.240(15) . ?
O6 C4 1.266(16) . ?
O5 C8 1.265(15) 2_667 ?
O4 C6 1.258(14) . ?
O4 U2 2.421(9) 2_666 ?
O3 C10 1.264(16) . ?
O2 C2 1.234(15) . ?
O2 U3 2.407(8) 2_667 ?
O1 C11 1.232(15) . ?
C12 O29 1.239(14) 2_666 ?
C8 O5 1.265(15) 2_667 ?
O35 C13 1.26(2) . ?
O34 C13 1.40(3) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O32 U6 O33 89.7(3) . . ?
O32 U6 O5 98.8(3) . . ?
O33 U6 O5 142.5(3) . . ?
O32 U6 O23 78.9(3) . . ?
O33 U6 O23 145.5(3) . . ?
O5 U6 O23 71.9(3) . . ?
O32 U6 O20 145.9(3) . . ?
O33 U6 O20 78.9(3) . . ?
O5 U6 O20 73.7(3) . . ?
O23 U6 O20 126.9(3) . . ?
O32 U6 O19 143.0(3) . . ?
O33 U6 O19 101.6(3) . . ?
O5 U6 O19 93.3(3) . . ?
O23 U6 O19 71.8(3) . . ?
O20 U6 O19 71.1(3) . . ?
O32 U6 O28 69.8(2) . . ?
O33 U6 O28 70.7(2) . . ?
O5 U6 O28 78.1(3) . . ?
O23 U6 O28 132.2(3) . . ?
O20 U6 O28 76.1(3) . . ?
O19 U6 O28 147.2(3) . . ?
O32 U6 O30 70.5(2) . . ?
O33 U6 O30 69.0(3) . . ?
O5 U6 O30 148.1(3) . . ?
O23 U6 O30 76.5(3) . . ?
O20 U6 O30 131.6(3) . . ?
O19 U6 O30 80.8(2) . . ?
O28 U6 O30 122.4(2) . . ?
O32 U6 U3 81.95(18) . . ?
O33 U6 U3 31.55(19) . . ?
O5 U6 U3 113.5(2) . . ?
O23 U6 U3 160.8(2) . . ?
O20 U6 U3 71.5(2) . . ?
O19 U6 U3 124.5(2) . . ?
O28 U6 U3 39.47(17) . . ?
O30 U6 U3 95.18(16) . . ?
O32 U6 U4 31.08(17) . . ?
O33 U6 U4 81.52(19) . . ?
O5 U6 U4 87.3(2) . . ?
O23 U6 U4 102.6(2) . . ?
O20 U6 U4 114.9(2) . . ?
O19 U6 U4 173.8(2) . . ?
O28 U6 U4 38.86(18) . . ?
O30 U6 U4 95.52(16) . . ?
U3 U6 U4 60.496(11) . . ?
O32 U6 U2 31.28(17) . . ?
O33 U6 U2 81.9(2) . . ?
O5 U6 U2 122.4(2) . . ?
O23 U6 U2 71.5(2) . . ?
O20 U6 U2 160.6(2) . . ?
O19 U6 U2 115.14(19) . . ?
O28 U6 U2 95.76(18) . . ?
O30 U6 U2 39.58(17) . . ?
U3 U6 U2 90.956(12) . . ?
U4 U6 U2 59.784(11) . . ?
O32 U6 U5 80.53(18) . . ?
O33 U6 U5 30.82(19) . . ?
O5 U6 U5 172.9(2) . . ?
O23 U6 U5 114.7(2) . . ?
O20 U6 U5 102.8(2) . . ?
O19 U6 U5 91.4(2) . . ?
O28 U6 U5 95.14(17) . . ?
O30 U6 U5 38.21(17) . . ?
U3 U6 U5 59.488(11) . . ?
U4 U6 U5 88.714(12) . . ?
U2 U6 U5 59.877(11) . . ?
O27 U5 O33 90.3(3) . . ?
O27 U5 O26 144.2(3) . . ?
O33 U5 O26 90.0(3) . . ?
O27 U5 O29 92.4(3) . . ?
O33 U5 O29 145.7(3) . . ?
O26 U5 O29 68.5(3) . . ?
O27 U5 O14 84.8(3) . . ?
O33 U5 O14 143.0(3) . . ?
O26 U5 O14 114.8(3) . . ?
O29 U5 O14 71.3(3) . . ?
O27 U5 O22 71.0(3) . . ?
O33 U5 O22 71.2(3) . . ?
O26 U5 O22 141.7(3) . . ?
O29 U5 O22 141.3(3) . . ?
O14 U5 O22 72.6(3) . . ?
O27 U5 O25 143.8(3) . . ?
O33 U5 O25 81.2(3) . . ?
O26 U5 O25 71.3(3) . . ?
O29 U5 O25 114.1(3) . . ?
O14 U5 O25 81.4(3) . . ?
O22 U5 O25 73.0(3) . . ?
O27 U5 O30 70.0(3) . . ?
O33 U5 O30 69.1(3) . . ?
O26 U5 O30 76.8(3) . . ?
O29 U5 O30 79.8(3) . . ?
O14 U5 O30 140.6(3) . . ?
O22 U5 O30 122.9(2) . . ?
O25 U5 O30 136.0(3) . . ?
O27 U5 U3 82.9(2) . . ?
O33 U5 U3 31.81(18) . . ?
O26 U5 U3 113.7(2) . . ?
O29 U5 U3 174.4(2) . . ?
O14 U5 U3 111.26(19) . . ?
O22 U5 U3 39.62(18) . . ?
O25 U5 U3 71.41(19) . . ?
O30 U5 U3 95.57(16) . . ?
O27 U5 U1 33.14(19) . . ?
O33 U5 U1 82.87(19) . . ?
O26 U5 U1 172.1(2) . . ?
O29 U5 U1 116.1(2) . . ?
O14 U5 U1 73.15(18) . . ?
O22 U5 U1 38.14(19) . . ?
O25 U5 U1 110.7(2) . . ?
O30 U5 U1 97.39(16) . . ?
U3 U5 U1 61.051(11) . . ?
O27 U5 U2 30.77(19) . . ?
O33 U5 U2 81.6(2) . . ?
O26 U5 U2 114.3(2) . . ?
O29 U5 U2 83.5(2) . . ?
O14 U5 U2 109.5(2) . . ?
O22 U5 U2 96.02(18) . . ?
O25 U5 U2 161.9(2) . . ?
O30 U5 U2 39.38(17) . . ?
U3 U5 U2 90.913(12) . . ?
U1 U5 U2 61.375(11) . . ?
O27 U5 U6 80.7(2) . . ?
O33 U5 U6 30.60(19) . . ?
O26 U5 U6 81.5(2) . . ?
O29 U5 U6 116.6(2) . . ?
O14 U5 U6 163.66(18) . . ?
O22 U5 U6 95.44(18) . . ?
O25 U5 U6 106.1(2) . . ?
O30 U5 U6 38.55(17) . . ?
U3 U5 U6 59.562(11) . . ?
U1 U5 U6 90.556(12) . . ?
U2 U5 U6 59.731(11) . . ?
O31 U4 O32 89.8(3) . . ?
O31 U4 O7 142.8(3) . . ?
O32 U4 O7 91.0(3) . . ?
O31 U4 O11 86.4(3) . . ?
O32 U4 O11 143.1(3) . . ?
O7 U4 O11 113.5(3) . . ?
O31 U4 O9 144.6(3) . . ?
O32 U4 O9 81.8(3) . . ?
O7 U4 O9 72.1(3) . . ?
O11 U4 O9 80.4(3) . . ?
O31 U4 O21 71.2(3) . . ?
O32 U4 O21 70.4(2) . . ?
O7 U4 O21 142.9(3) . . ?
O11 U4 O21 73.6(3) . . ?
O9 U4 O21 73.6(3) . . ?
O31 U4 O18 88.8(3) . . ?
O32 U4 O18 144.3(3) . . ?
O7 U4 O18 69.6(3) . . ?
O11 U4 O18 72.4(3) . . ?
O9 U4 O18 117.6(3) . . ?
O21 U4 O18 141.4(3) . . ?
O31 U4 O28 69.2(2) . . ?
O32 U4 O28 69.3(2) . . ?
O7 U4 O28 76.4(3) . . ?
O11 U4 O28 140.9(3) . . ?
O9 U4 O28 136.3(3) . . ?
O21 U4 O28 122.3(2) . . ?
O18 U4 O28 76.9(3) . . ?
O31 U4 U1 32.68(19) . . ?
O32 U4 U1 82.97(18) . . ?
O7 U4 U1 172.1(2) . . ?
O11 U4 U1 74.2(2) . . ?
O9 U4 U1 111.9(2) . . ?
O21 U4 U1 38.95(18) . . ?
O18 U4 U1 112.8(2) . . ?
O28 U4 U1 96.63(16) . . ?
O31 U4 U2 82.95(19) . . ?
O32 U4 U2 31.75(18) . . ?
O7 U4 U2 114.9(2) . . ?
O11 U4 U2 111.5(2) . . ?
O9 U4 U2 71.88(19) . . ?
O21 U4 U2 38.96(17) . . ?
O18 U4 U2 170.5(2) . . ?
O28 U4 U2 95.77(17) . . ?
U1 U4 U2 61.654(11) . . ?
O31 U4 U6 80.79(18) . . ?
O32 U4 U6 30.87(18) . . ?
O7 U4 U6 81.1(2) . . ?
O11 U4 U6 165.3(2) . . ?
O9 U4 U6 106.2(2) . . ?
O21 U4 U6 95.39(17) . . ?
O18 U4 U6 114.1(2) . . ?
O28 U4 U6 38.54(17) . . ?
U1 U4 U6 91.134(12) . . ?
U2 U4 U6 60.094(11) . . ?
O31 U4 U3 30.61(19) . . ?
O32 U4 U3 80.78(18) . . ?
O7 U4 U3 113.3(2) . . ?
O11 U4 U3 111.1(2) . . ?
O9 U4 U3 161.82(19) . . ?
O21 U4 U3 95.65(18) . . ?
O18 U4 U3 80.1(2) . . ?
O28 U4 U3 38.75(17) . . ?
U1 U4 U3 60.764(11) . . ?
U2 U4 U3 90.485(12) . . ?
U6 U4 U3 59.384(11) . . ?
O33 U3 O31 89.4(3) . . ?
O33 U3 O3 143.4(3) . . ?
O31 U3 O3 82.6(3) . . ?
O33 U3 O2 144.1(3) . 2_667 ?
O31 U3 O2 96.9(3) . 2_667 ?
O3 U3 O2 72.5(3) . 2_667 ?
O33 U3 O12 81.7(3) . . ?
O31 U3 O12 140.6(3) . . ?
O3 U3 O12 82.2(3) . . ?
O2 U3 O12 112.6(3) 2_667 . ?
O33 U3 O24 79.9(3) . . ?
O31 U3 O24 142.8(3) . . ?
O3 U3 O24 125.7(3) . . ?
O2 U3 O24 73.7(3) 2_667 . ?
O12 U3 O24 73.2(3) . . ?
O33 U3 O28 70.5(3) . . ?
O31 U3 O28 68.7(2) . . ?
O3 U3 O28 136.5(3) . . ?
O2 U3 O28 79.1(3) 2_667 . ?
O12 U3 O28 140.1(3) . . ?
O24 U3 O28 74.2(3) . . ?
O33 U3 O22 70.3(3) . . ?
O31 U3 O22 68.8(3) . . ?
O3 U3 O22 73.5(3) . . ?
O2 U3 O22 144.5(3) 2_667 . ?
O12 U3 O22 72.1(3) . . ?
O24 U3 O22 136.7(3) . . ?
O28 U3 O22 121.1(3) . . ?
O33 U3 U6 31.64(19) . . ?
O31 U3 U6 81.10(17) . . ?
O3 U3 U6 163.0(2) . . ?
O2 U3 U6 114.6(2) 2_667 . ?
O12 U3 U6 107.5(2) . . ?
O24 U3 U6 71.2(2) . . ?
O28 U3 U6 39.09(17) . . ?
O22 U3 U6 95.72(18) . . ?
O33 U3 U5 32.13(18) . . ?
O31 U3 U5 80.99(18) . . ?
O3 U3 U5 111.3(2) . . ?
O2 U3 U5 175.2(2) 2_667 . ?
O12 U3 U5 71.2(2) . . ?
O24 U3 U5 105.3(2) . . ?
O28 U3 U5 96.19(17) . . ?
O22 U3 U5 38.47(18) . . ?
U6 U3 U5 60.950(11) . . ?
O33 U3 U4 81.2(2) . . ?
O31 U3 U4 30.10(17) . . ?
O3 U3 U4 106.5(2) . . ?
O2 U3 U4 86.8(2) 2_667 . ?
O12 U3 U4 160.5(2) . . ?
O24 U3 U4 112.7(2) . . ?
O28 U3 U4 38.69(18) . . ?
O22 U3 U4 93.32(18) . . ?
U6 U3 U4 60.120(11) . . ?
U5 U3 U4 89.323(12) . . ?
O33 U3 U1 81.9(2) . . ?
O31 U3 U1 31.55(18) . . ?
O3 U3 U1 72.8(2) . . ?
O2 U3 U1 120.1(3) 2_667 . ?
O12 U3 U1 109.1(2) . . ?
O24 U3 U1 161.1(2) . . ?
O28 U3 U1 94.99(18) . . ?
O22 U3 U1 37.55(18) . . ?
U6 U3 U1 90.599(12) . . ?
U5 U3 U1 59.740(11) . . ?
U4 U3 U1 59.125(11) . . ?
O27 U2 O32 88.4(3) . . ?
O27 U2 O6 140.0(3) . . ?
O32 U2 O6 80.7(3) . . ?
O27 U2 O4 90.1(3) . 2_666 ?
O32 U2 O4 141.5(3) . 2_666 ?
O6 U2 O4 121.7(3) . 2_666 ?
O27 U2 O10 141.2(3) . . ?
O32 U2 O10 79.5(3) . . ?
O6 U2 O10 74.3(3) . . ?
O4 U2 O10 77.8(3) 2_666 . ?
O27 U2 O21 68.7(3) . . ?
O32 U2 O21 69.8(3) . . ?
O6 U2 O21 71.4(3) . . ?
O4 U2 O21 143.5(3) 2_666 . ?
O10 U2 O21 136.9(3) . . ?
O27 U2 O8 79.6(3) . . ?
O32 U2 O8 142.5(3) . . ?
O6 U2 O8 86.0(3) . . ?
O4 U2 O8 74.5(3) 2_666 . ?
O10 U2 O8 130.0(3) . . ?
O21 U2 O8 72.7(3) . . ?
O27 U2 O30 68.4(2) . . ?
O32 U2 O30 69.9(2) . . ?
O6 U2 O30 139.0(3) . . ?
O4 U2 O30 73.8(3) 2_666 . ?
O10 U2 O30 72.8(3) . . ?
O21 U2 O30 120.6(2) . . ?
O8 U2 O30 134.3(3) . . ?
O27 U2 O35 140.0(4) . . ?
O32 U2 O35 131.6(3) . . ?
O6 U2 O35 61.3(4) . . ?
O4 U2 O35 60.5(4) 2_666 . ?
O10 U2 O35 62.9(4) . . ?
O21 U2 O35 118.6(3) . . ?
O8 U2 O35 67.3(4) . . ?
O30 U2 O35 120.8(3) . . ?
O27 U2 U4 80.58(19) . . ?
O32 U2 U4 31.66(18) . . ?
O6 U2 U4 70.0(2) . . ?
O4 U2 U4 168.0(2) 2_666 . ?
O10 U2 U4 104.7(2) . . ?
O21 U2 U4 38.47(18) . . ?
O8 U2 U4 110.9(2) . . ?
O30 U2 U4 95.51(16) . . ?
O35 U2 U4 131.3(3) . . ?
O27 U2 U6 80.69(18) . . ?
O32 U2 U6 30.98(18) . . ?
O6 U2 U6 105.8(2) . . ?
O4 U2 U6 111.1(2) 2_666 . ?
O10 U2 U6 70.01(19) . . ?
O21 U2 U6 94.97(18) . . ?
O8 U2 U6 159.6(2) . . ?
O30 U2 U6 39.21(16) . . ?
O35 U2 U6 132.9(3) . . ?
U4 U2 U6 60.122(11) . . ?
O27 U2 U5 29.92(18) . . ?
O32 U2 U5 80.78(18) . . ?
O6 U2 U5 159.2(2) . . ?
O4 U2 U5 79.0(2) 2_666 . ?
O10 U2 U5 111.3(2) . . ?
O21 U2 U5 93.25(18) . . ?
O8 U2 U5 103.2(2) . . ?
O30 U2 U5 38.68(16) . . ?
O35 U2 U5 139.5(3) . . ?
U4 U2 U5 89.197(12) . . ?
U6 U2 U5 60.392(11) . . ?
O31 U1 O27 87.4(3) . . ?
O31 U1 O22 69.0(3) . . ?
O27 U1 O22 68.7(3) . . ?
O31 U1 O21 69.7(3) . . ?
O27 U1 O21 67.8(3) . . ?
O22 U1 O21 120.0(3) . . ?
O31 U1 O1 140.7(3) . . ?
O27 U1 O1 78.5(3) . . ?
O22 U1 O1 71.6(3) . . ?
O21 U1 O1 133.8(3) . . ?
O31 U1 O15 77.4(3) . . ?
O27 U1 O15 139.0(3) . . ?
O22 U1 O15 70.3(3) . . ?
O21 U1 O15 136.5(3) . . ?
O1 U1 O15 89.6(3) . . ?
O31 U1 O13 78.8(3) . . ?
O27 U1 O13 138.9(3) . . ?
O22 U1 O13 136.9(3) . . ?
O21 U1 O13 71.1(3) . . ?
O1 U1 O13 133.8(3) . . ?
O15 U1 O13 75.3(3) . . ?
O31 U1 O16 139.9(3) . . ?
O27 U1 O16 79.4(3) . . ?
O22 U1 O16 136.3(3) . . ?
O21 U1 O16 70.2(3) . . ?
O1 U1 O16 73.3(3) . . ?
O15 U1 O16 134.5(3) . . ?
O13 U1 O16 86.7(3) . . ?
O31 U1 O17 133.8(3) . . ?
O27 U1 O17 138.7(3) . . ?
O22 U1 O17 117.4(3) . . ?
O21 U1 O17 122.5(3) . . ?
O1 U1 O17 67.0(3) . . ?
O15 U1 O17 64.8(3) . . ?
O13 U1 O17 67.0(3) . . ?
O16 U1 O17 69.8(3) . . ?
O31 U1 U4 31.54(18) . . ?
O27 U1 U4 80.10(19) . . ?
O22 U1 U4 95.01(18) . . ?
O21 U1 U4 38.63(18) . . ?
O1 U1 U4 157.8(2) . . ?
O15 U1 U4 102.8(2) . . ?
O13 U1 U4 68.0(2) . . ?
O16 U1 U4 108.5(2) . . ?
O17 U1 U4 135.0(2) . . ?
O31 U1 U5 80.09(17) . . ?
O27 U1 U5 31.17(19) . . ?
O22 U1 U5 37.84(18) . . ?
O21 U1 U5 93.78(17) . . ?
O1 U1 U5 68.9(2) . . ?
O15 U1 U5 108.1(2) . . ?
O13 U1 U5 157.3(2) . . ?
O16 U1 U5 104.4(2) . . ?
O17 U1 U5 135.2(2) . . ?
U4 U1 U5 89.590(12) . . ?
O31 U1 U3 30.97(18) . . ?
O27 U1 U3 79.88(18) . . ?
O22 U1 U3 38.35(18) . . ?
O21 U1 U3 94.74(18) . . ?
O1 U1 U3 109.8(2) . . ?
O15 U1 U3 67.5(2) . . ?
O13 U1 U3 104.2(2) . . ?
O16 U1 U3 157.9(2) . . ?
O17 U1 U3 132.1(2) . . ?
U4 U1 U3 60.111(11) . . ?
U5 U1 U3 59.209(11) . . ?
U3 O33 U6 116.8(3) . . ?
U3 O33 U5 116.1(3) . . ?
U6 O33 U5 118.6(3) . . ?
U6 O32 U4 118.1(3) . . ?
U6 O32 U2 117.7(3) . . ?
U4 O32 U2 116.6(3) . . ?
U4 O31 U3 119.3(3) . . ?
U4 O31 U1 115.8(3) . . ?
U3 O31 U1 117.5(3) . . ?
U5 O30 U6 103.2(3) . . ?
U5 O30 U2 101.9(3) . . ?
U6 O30 U2 101.2(2) . . ?
C12 O29 U5 142.6(8) 2_666 . ?
U6 O28 U3 101.4(2) . . ?
U6 O28 U4 102.6(3) . . ?
U3 O28 U4 102.6(3) . . ?
U5 O27 U2 119.3(3) . . ?
U5 O27 U1 115.7(3) . . ?
U2 O27 U1 117.6(3) . . ?
C6 O26 U5 142.6(8) . . ?
C3 O25 U5 134.4(8) . . ?
C7 O24 U3 134.9(8) . . ?
C5 O23 U6 135.8(8) . . ?
U5 O22 U1 104.0(3) . . ?
U5 O22 U3 101.9(3) . . ?
U1 O22 U3 104.1(3) . . ?
U4 O21 U1 102.4(3) . . ?
U4 O21 U2 102.6(3) . . ?
U1 O21 U2 105.5(3) . . ?
C7 O20 U6 135.7(8) . . ?
C12 O19 U6 135.0(8) . . ?
C8 O18 U4 144.6(9) . . ?
C9 O16 U1 138.7(9) . . ?
C10 O15 U1 140.0(9) . . ?
C11 O14 U5 132.7(7) . . ?
C1 O13 U1 139.2(8) . . ?
C3 O12 U3 136.9(8) . . ?
C1 O11 U4 132.2(8) . . ?
C5 O10 U2 136.2(7) . . ?
C4 O9 U4 134.7(8) . . ?
C9 O8 U2 135.6(9) . . ?
C2 O7 U4 143.2(9) . . ?
C4 O6 U2 137.6(8) . . ?
C8 O5 U6 137.6(9) 2_667 . ?
C6 O4 U2 138.4(9) . 2_666 ?
C10 O3 U3 133.0(8) . . ?
C2 O2 U3 137.7(8) . 2_667 ?
C11 O1 U1 137.7(8) . . ?
O20 C7 O24 126.0(11) . . ?
O26 C6 O4 124.5(12) . . ?
O23 C5 O10 126.0(11) . . ?
O6 C4 O9 125.7(12) . . ?
O12 C3 O25 125.9(12) . . ?
O7 C2 O2 124.9(13) . . ?
O13 C1 O11 125.9(11) . . ?
O29 C12 O19 125.0(12) 2_666 . ?
O14 C11 O1 126.9(11) . . ?
O15 C10 O3 126.2(12) . . ?
O16 C9 O8 124.5(13) . . ?
O18 C8 O5 124.5(13) . 2_667 ?
C13 O35 U2 137.2(16) . . ?
O35 C13 O34 115(2) . . ?

_refine_diff_density_max         5.356
_refine_diff_density_min         -2.597
_refine_diff_density_rms         0.382

_shelxl_version_number           2014-3



####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_C29H33N3O36U6
_database_code_depnum_ccdc_archive 'CCDC 1850749'
_audit_update_record             
;
2018-06-21 deposited with the CCDC.
2018-10-08 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            'Uranium formic acid pyridine'
_chemical_melting_point          N/a
_chemical_formula_moiety         'C29 H23 N O36 U6, 2(C5 H5 N)'
_chemical_formula_sum            'C29 H33 N3 O36 U6'
_chemical_formula_weight         2427.76

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        'C 2/c'
_space_group_name_Hall           '-C 2yc'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   20.458(3)
_cell_length_b                   15.473(3)
_cell_length_c                   15.918(2)
_cell_angle_alpha                90
_cell_angle_beta                 107.718(10)
_cell_angle_gamma                90
_cell_volume                     4799.9(13)
_cell_formula_units_Z            4
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    9852
_cell_measurement_theta_min      2.34
_cell_measurement_theta_max      27.44

_exptl_crystal_description       Rodlike
_exptl_crystal_colour            Green
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.360
_exptl_crystal_F_000             4272
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.060
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.020
_exptl_absorpt_coefficient_mu    20.283
_shelx_estimated_absorpt_T_min   0.376
_shelx_estimated_absorpt_T_max   0.687
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.393
_exptl_absorpt_correction_T_max  0.667
_exptl_absorpt_process_details   SHELTXPREP

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'Turbo X-ray Source'
_diffrn_measurement_device_type  'Bruker APEX-III '
_diffrn_measurement_method       '0.5 wide w/ exposures'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            108607
_diffrn_reflns_av_unetI/netI     0.0407
_diffrn_reflns_av_R_equivalents  0.1051
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_theta_min         2.633
_diffrn_reflns_theta_max         27.650
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measured_fraction_theta_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.993
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_point_group_measured_fraction_full 0.998
_reflns_number_total             5569
_reflns_number_gt                4179
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker APEX3'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
;
 ?
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0377P)²+17.7193P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         5569
_refine_ls_number_parameters     336
_refine_ls_number_restraints     6
_refine_ls_R_factor_all          0.0548
_refine_ls_R_factor_gt           0.0296
_refine_ls_wR_factor_ref         0.0667
_refine_ls_wR_factor_gt          0.0585
_refine_ls_goodness_of_fit_ref   0.951
_refine_ls_restrained_S_all      0.951
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.5000 0.03966(2) 0.2500 0.00927(9) Uani 1 2 d S T P . .
U2 U 0.61971(2) -0.13354(2) 0.21193(2) 0.00927(7) Uani 1 1 d . . . . .
U3 U 0.42954(2) -0.13565(2) 0.07628(2) 0.00892(7) Uani 1 1 d . . . . .
U4 U 0.5000 -0.31107(2) 0.2500 0.00951(9) Uani 1 2 d S T P . .
O9 O 0.3992(2) 0.0005(3) -0.0059(3) 0.0162(11) Uani 1 1 d . . . . .
O8 O 0.3130(2) -0.1372(3) -0.0004(3) 0.0214(11) Uani 1 1 d . . . . .
O7 O 0.5275(2) -0.0364(3) 0.1314(3) 0.0097(10) Uani 1 1 d . . . . .
H7B H 0.5378 0.0002 0.0868 0.012 Uiso 1 1 calc R U . . .
O6 O 0.4141(3) -0.2738(3) 0.0003(3) 0.0196(11) Uani 1 1 d . . . . .
O5 O 0.5977(2) -0.3731(3) 0.2156(3) 0.0170(11) Uani 1 1 d . . . . .
O4 O 0.4797(2) -0.1272(3) -0.0407(3) 0.0169(11) Uani 1 1 d . . . . .
O3 O 0.7309(2) -0.1361(3) 0.3073(3) 0.0216(11) Uani 1 1 d . . . . .
O2 O 0.4510(2) -0.3744(3) 0.1058(3) 0.0170(11) Uani 1 1 d . . . . .
O1 O 0.5214(2) -0.2049(3) 0.1618(3) 0.0099(10) Uani 1 1 d . . . . .
O16 O 0.4627(2) 0.1478(3) 0.1360(3) 0.0148(10) Uani 1 1 d . . . . .
O15 O 0.4197(2) -0.0597(3) 0.1912(3) 0.0091(10) Uani 1 1 d . . . . .
O14 O 0.6480(2) -0.1203(3) 0.0763(3) 0.0163(11) Uani 1 1 d . . . . .
O13 O 0.3934(2) -0.2291(3) 0.1732(3) 0.0114(10) Uani 1 1 d . . . . .
H13B H 0.3533 -0.2649 0.1448 0.014 Uiso 1 1 calc R U . . .
O12 O 0.6035(2) 0.1107(3) 0.2404(3) 0.0165(11) Uani 1 1 d . . . . .
O11 O 0.6646(2) -0.2720(3) 0.1825(3) 0.0186(11) Uani 1 1 d . . . . .
O10 O 0.6730(2) 0.0095(3) 0.2125(3) 0.0176(11) Uani 1 1 d . . . . .
O17 O 0.2067(3) -0.1577(3) -0.0873(4) 0.0312(14) Uani 1 1 d . . . . .
N2 N 0.5000 -0.4901(5) 0.2500 0.0147(18) Uani 1 2 d S T P . .
C5 C 0.4246(4) -0.3502(4) 0.0280(5) 0.0176(16) Uani 1 1 d . . . . .
H5A H 0.4110 -0.3935 -0.0142 0.021 Uiso 1 1 calc R U . . .
C4 C 0.3560(4) 0.0578(5) -0.0222(4) 0.0175(16) Uani 1 1 d . . . . .
H4A H 0.3231 0.0558 0.0073 0.021 Uiso 1 1 calc R U . . .
C2 C 0.4827(3) 0.1708(5) 0.0725(5) 0.0154(15) Uani 1 1 d . . . . .
H2A H 0.4684 0.2245 0.0473 0.018 Uiso 1 1 calc R U . . .
C1 C 0.2671(4) -0.1766(5) -0.0604(5) 0.0229(17) Uani 1 1 d . . . . .
H1A H 0.2811 -0.2244 -0.0860 0.027 Uiso 1 1 calc R U . . .
C3 C 0.6555(4) 0.0861(5) 0.2222(5) 0.0187(16) Uani 1 1 d . . . . .
H3A H 0.6849 0.1293 0.2148 0.022 Uiso 1 1 calc R U . . .
O18 O 0.8223(3) -0.0489(4) 0.3465(4) 0.0334(14) Uani 1 1 d . . . . .
C8 C 0.6489(4) -0.3483(5) 0.1962(5) 0.0212(17) Uani 1 1 d . . . . .
H8A H 0.6793 -0.3911 0.1911 0.025 Uiso 1 1 calc R U . . .
C7 C 0.5191(4) -0.5350(5) 0.1907(5) 0.0219(17) Uani 1 1 d . . . . .
H7A H 0.5325 -0.5048 0.1481 0.026 Uiso 1 1 calc R U . . .
C6 C 0.7724(4) -0.0840(6) 0.3600(5) 0.033(2) Uani 1 1 d . . . . .
H6A H 0.7642 -0.0716 0.4131 0.040 Uiso 1 1 calc R U . . .
C10 C 0.5202(4) -0.6246(5) 0.1884(5) 0.0262(19) Uani 1 1 d . . . . .
H10A H 0.5345 -0.6529 0.1456 0.031 Uiso 1 1 calc R U . . .
C14 C 0.8230(3) 0.0955(5) 0.6797(5) 0.0171(15) Uani 1 1 d . . . . .
H14A H 0.8209 0.0694 0.7315 0.020 Uiso 1 1 calc R U . . .
C15 C 0.8167(4) 0.1801(6) 0.6734(6) 0.041(2) Uani 1 1 d . . . . .
H15A H 0.8074 0.2113 0.7184 0.049 Uiso 1 1 calc R U . . .
N1 N 0.8237(4) 0.2236(6) 0.5997(6) 0.063(3) Uani 1 1 d . . . . .
C12 C 0.8390(5) 0.0833(7) 0.5419(6) 0.046(3) Uani 1 1 d . . . . .
H12A H 0.8470 0.0493 0.4978 0.055 Uiso 1 1 calc R U . . .
C13 C 0.8321(5) 0.0451(6) 0.6168(6) 0.041(2) Uani 1 1 d . . . . .
H13A H 0.8338 -0.0147 0.6232 0.049 Uiso 1 1 calc R U . . .
C9 C 0.5000 -0.6715(7) 0.2500 0.032(3) Uani 1 2 d S TU P . .
H9A H 0.5000 -0.7316 0.2500 0.038 Uiso 1 2 calc R U P . .
C11 C 0.8340(4) 0.1724(7) 0.5319(6) 0.037(2) Uani 1 1 d . . . . .
H11A H 0.8373 0.1982 0.4805 0.045 Uiso 1 1 calc R U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
U1 O15 2.238(4) . ?
U1 O15 2.238(4) 2_655 ?
U1 O16 2.415(4) 2_655 ?
U1 O16 2.415(4) . ?
U1 O12 2.431(5) 2_655 ?
U1 O12 2.431(5) . ?
U1 O7 2.432(4) . ?
U1 O7 2.432(4) 2_655 ?
U1 U2 3.8014(5) 2_655 ?
U1 U2 3.8015(6) . ?
U1 U3 3.8284(6) . ?
U1 U3 3.8284(6) 2_655 ?
U2 O1 2.219(4) . ?
U2 O15 2.255(4) 2_655 ?
U2 O3 2.319(5) . ?
U2 O14 2.409(5) . ?
U2 O11 2.432(5) . ?
U2 O13 2.429(4) 2_655 ?
U2 O7 2.448(4) . ?
U2 O10 2.466(5) . ?
U2 U3 3.8013(6) 2_655 ?
U2 U3 3.8325(7) . ?
U2 U4 3.8489(6) . ?
U3 O1 2.230(4) . ?
U3 O15 2.234(4) . ?
U3 O8 2.325(5) . ?
U3 O4 2.388(4) . ?
U3 O13 2.390(4) . ?
U3 O6 2.428(5) . ?
U3 O9 2.457(4) . ?
U3 O7 2.464(4) . ?
U3 U2 3.8013(6) 2_655 ?
U3 U4 3.8296(6) . ?
U4 O1 2.288(4) . ?
U4 O1 2.288(4) 2_655 ?
U4 O2 2.415(5) 2_655 ?
U4 O2 2.416(5) . ?
U4 O5 2.425(5) 2_655 ?
U4 O5 2.425(5) . ?
U4 O13 2.497(4) 2_655 ?
U4 O13 2.497(4) . ?
U4 N2 2.769(8) . ?
U4 U3 3.8297(6) 2_655 ?
O9 C4 1.224(8) . ?
O8 C1 1.273(9) . ?
O6 C5 1.257(8) . ?
O5 C8 1.240(9) . ?
O4 C2 1.239(8) 5_655 ?
O3 C6 1.282(9) . ?
O2 C5 1.248(8) . ?
O16 C2 1.253(8) . ?
O15 U2 2.255(4) 2_655 ?
O14 C4 1.281(8) 5_655 ?
O13 U2 2.429(4) 2_655 ?
O12 C3 1.244(8) . ?
O11 C8 1.260(8) . ?
O10 C3 1.261(8) . ?
O17 C1 1.213(9) . ?
N2 C7 1.324(8) 2_655 ?
N2 C7 1.324(8) . ?
C4 O14 1.281(8) 5_655 ?
C2 O4 1.239(8) 5_655 ?
O18 C6 1.231(9) . ?
C7 C10 1.387(10) . ?
C10 C9 1.380(10) . ?
C14 C15 1.317(12) . ?
C14 C13 1.326(11) . ?
C15 N1 1.398(12) . ?
N1 C11 1.404(12) . ?
C12 C13 1.377(13) . ?
C12 C11 1.389(14) . ?
C9 C10 1.380(10) 2_655 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O15 U1 O15 93.2(2) . 2_655 ?
O15 U1 O16 144.53(15) . 2_655 ?
O15 U1 O16 97.93(15) 2_655 2_655 ?
O15 U1 O16 97.93(15) . . ?
O15 U1 O16 144.54(15) 2_655 . ?
O16 U1 O16 92.3(2) 2_655 . ?
O15 U1 O12 78.13(15) . 2_655 ?
O15 U1 O12 145.82(15) 2_655 2_655 ?
O16 U1 O12 73.83(16) 2_655 2_655 ?
O16 U1 O12 69.63(15) . 2_655 ?
O15 U1 O12 145.82(15) . . ?
O15 U1 O12 78.13(15) 2_655 . ?
O16 U1 O12 69.64(15) 2_655 . ?
O16 U1 O12 73.83(16) . . ?
O12 U1 O12 126.2(2) 2_655 . ?
O15 U1 O7 69.90(14) . . ?
O15 U1 O7 71.23(14) 2_655 . ?
O16 U1 O7 145.50(15) 2_655 . ?
O16 U1 O7 81.18(14) . . ?
O12 U1 O7 132.79(15) 2_655 . ?
O12 U1 O7 76.03(15) . . ?
O15 U1 O7 71.23(14) . 2_655 ?
O15 U1 O7 69.90(14) 2_655 2_655 ?
O16 U1 O7 81.18(14) 2_655 2_655 ?
O16 U1 O7 145.50(15) . 2_655 ?
O12 U1 O7 76.03(15) 2_655 2_655 ?
O12 U1 O7 132.79(15) . 2_655 ?
O7 U1 O7 122.1(2) . 2_655 ?
O15 U1 U2 32.35(10) . 2_655 ?
O15 U1 U2 82.86(11) 2_655 2_655 ?
O16 U1 U2 116.12(11) 2_655 2_655 ?
O16 U1 U2 122.45(11) . 2_655 ?
O12 U1 U2 72.13(11) 2_655 2_655 ?
O12 U1 U2 160.81(11) . 2_655 ?
O7 U1 U2 95.44(10) . 2_655 ?
O7 U1 U2 38.97(10) 2_655 2_655 ?
O15 U1 U2 82.86(11) . . ?
O15 U1 U2 32.35(10) 2_655 . ?
O16 U1 U2 122.45(11) 2_655 . ?
O16 U1 U2 116.12(11) . . ?
O12 U1 U2 160.81(11) 2_655 . ?
O12 U1 U2 72.13(11) . . ?
O7 U1 U2 38.97(10) . . ?
O7 U1 U2 95.44(10) 2_655 . ?
U2 U1 U2 90.346(17) 2_655 . ?
O15 U1 U3 31.09(10) . . ?
O15 U1 U3 83.24(11) 2_655 . ?
O16 U1 U3 175.62(11) 2_655 . ?
O16 U1 U3 89.12(11) . . ?
O12 U1 U3 102.84(11) 2_655 . ?
O12 U1 U3 114.74(11) . . ?
O7 U1 U3 38.85(10) . . ?
O7 U1 U3 95.32(10) 2_655 . ?
U2 U1 U3 59.763(11) 2_655 . ?
U2 U1 U3 60.304(12) . . ?
O15 U1 U3 83.25(11) . 2_655 ?
O15 U1 U3 31.09(10) 2_655 2_655 ?
O16 U1 U3 89.12(11) 2_655 2_655 ?
O16 U1 U3 175.62(11) . 2_655 ?
O12 U1 U3 114.74(11) 2_655 2_655 ?
O12 U1 U3 102.84(11) . 2_655 ?
O7 U1 U3 95.32(10) . 2_655 ?
O7 U1 U3 38.86(10) 2_655 2_655 ?
U2 U1 U3 60.305(12) 2_655 2_655 ?
U2 U1 U3 59.762(12) . 2_655 ?
U3 U1 U3 89.771(17) . 2_655 ?
O1 U2 O15 91.39(16) . 2_655 ?
O1 U2 O3 145.91(16) . . ?
O15 U2 O3 92.54(17) 2_655 . ?
O1 U2 O14 99.15(16) . . ?
O15 U2 O14 143.44(15) 2_655 . ?
O3 U2 O14 97.62(17) . . ?
O1 U2 O11 81.20(16) . . ?
O15 U2 O11 144.32(16) 2_655 . ?
O3 U2 O11 76.02(17) . . ?
O14 U2 O11 72.18(15) . . ?
O1 U2 O13 70.85(15) . 2_655 ?
O15 U2 O13 69.46(15) 2_655 2_655 ?
O3 U2 O13 78.95(16) . 2_655 ?
O14 U2 O13 146.98(15) . 2_655 ?
O11 U2 O13 75.16(15) . 2_655 ?
O1 U2 O7 69.32(15) . . ?
O15 U2 O7 70.65(14) 2_655 . ?
O3 U2 O7 143.10(16) . . ?
O14 U2 O7 80.53(14) . . ?
O11 U2 O7 135.72(15) . . ?
O13 U2 O7 121.58(14) 2_655 . ?
O1 U2 O10 143.03(16) . . ?
O15 U2 O10 78.02(15) 2_655 . ?
O3 U2 O10 70.64(17) . . ?
O14 U2 O10 72.55(15) . . ?
O11 U2 O10 126.78(15) . . ?
O13 U2 O10 133.93(15) 2_655 . ?
O7 U2 O10 73.76(15) . . ?
O1 U2 U3 81.88(11) . 2_655 ?
O15 U2 U3 31.98(11) 2_655 2_655 ?
O3 U2 U3 83.76(13) . 2_655 ?
O14 U2 U3 175.41(10) . 2_655 ?
O11 U2 U3 112.41(11) . 2_655 ?
O13 U2 U3 37.56(10) 2_655 2_655 ?
O7 U2 U3 95.73(10) . 2_655 ?
O10 U2 U3 103.92(11) . 2_655 ?
O1 U2 U1 81.39(11) . . ?
O15 U2 U1 32.07(10) 2_655 . ?
O3 U2 U1 117.31(13) . . ?
O14 U2 U1 115.17(10) . . ?
O11 U2 U1 162.03(11) . . ?
O13 U2 U1 94.87(10) 2_655 . ?
O7 U2 U1 38.68(10) . . ?
O10 U2 U1 70.86(11) . . ?
U3 U2 U1 60.471(8) 2_655 . ?
O1 U2 U3 30.62(11) . . ?
O15 U2 U3 82.93(11) 2_655 . ?
O3 U2 U3 173.71(13) . . ?
O14 U2 U3 88.60(11) . . ?
O11 U2 U3 105.20(11) . . ?
O13 U2 U3 95.33(10) 2_655 . ?
O7 U2 U3 38.86(10) . . ?
O10 U2 U3 112.42(11) . . ?
U3 U2 U3 90.114(14) 2_655 . ?
U1 U2 U3 60.196(9) . . ?
O1 U2 U4 31.90(11) . . ?
O15 U2 U4 82.93(11) 2_655 . ?
O3 U2 U4 115.42(12) . . ?
O14 U2 U4 122.69(11) . . ?
O11 U2 U4 72.40(11) . . ?
O13 U2 U4 39.24(10) 2_655 . ?
O7 U2 U4 95.42(10) . . ?
O10 U2 U4 160.34(11) . . ?
U3 U2 U4 60.075(8) 2_655 . ?
U1 U2 U4 90.361(15) . . ?
U3 U2 U4 59.809(9) . . ?
O1 U3 O15 91.26(16) . . ?
O1 U3 O8 148.71(16) . . ?
O15 U3 O8 95.83(17) . . ?
O1 U3 O4 91.15(16) . . ?
O15 U3 O4 141.02(15) . . ?
O8 U3 O4 101.91(17) . . ?
O1 U3 O13 71.57(15) . . ?
O15 U3 O13 70.52(16) . . ?
O8 U3 O13 82.18(16) . . ?
O4 U3 O13 145.82(15) . . ?
O1 U3 O6 80.72(16) . . ?
O15 U3 O6 147.13(16) . . ?
O8 U3 O6 76.85(17) . . ?
O4 U3 O6 71.41(16) . . ?
O13 U3 O6 76.72(15) . . ?
O1 U3 O9 139.98(15) . . ?
O15 U3 O9 85.09(16) . . ?
O8 U3 O9 71.15(16) . . ?
O4 U3 O9 68.70(16) . . ?
O13 U3 O9 141.71(15) . . ?
O6 U3 O9 121.05(16) . . ?
O1 U3 O7 68.85(15) . . ?
O15 U3 O7 69.36(14) . . ?
O8 U3 O7 141.84(15) . . ?
O4 U3 O7 75.38(15) . . ?
O13 U3 O7 121.65(14) . . ?
O6 U3 O7 133.93(15) . . ?
O9 U3 O7 72.63(15) . . ?
O1 U3 U2 82.20(11) . 2_655 ?
O15 U3 U2 32.32(11) . 2_655 ?
O8 U3 U2 87.69(13) . 2_655 ?
O4 U3 U2 169.77(11) . 2_655 ?
O13 U3 U2 38.28(11) . 2_655 ?
O6 U3 U2 114.82(11) . 2_655 ?
O9 U3 U2 111.89(11) . 2_655 ?
O7 U3 U2 94.90(10) . 2_655 ?
O1 U3 U1 80.63(11) . . ?
O15 U3 U1 31.14(11) . . ?
O8 U3 U1 119.16(13) . . ?
O4 U3 U1 111.59(11) . . ?
O13 U3 U1 94.85(10) . . ?
O6 U3 U1 161.17(11) . . ?
O9 U3 U1 75.87(11) . . ?
O7 U3 U1 38.26(10) . . ?
U2 U3 U1 59.766(9) 2_655 . ?
O1 U3 U4 32.52(11) . . ?
O15 U3 U4 83.65(11) . . ?
O8 U3 U4 118.20(12) . . ?
O4 U3 U4 116.43(11) . . ?
O13 U3 U4 39.40(10) . . ?
O6 U3 U4 72.48(11) . . ?
O9 U3 U4 166.04(11) . . ?
O7 U3 U4 95.62(10) . . ?
U2 U3 U4 60.580(9) 2_655 . ?
U1 U3 U4 90.249(15) . . ?
O1 U3 U2 30.45(11) . . ?
O15 U3 U2 82.16(11) . . ?
O8 U3 U2 177.56(13) . . ?
O4 U3 U2 80.53(12) . . ?
O13 U3 U2 95.83(10) . . ?
O6 U3 U2 104.10(12) . . ?
O9 U3 U2 109.94(11) . . ?
O7 U3 U2 38.56(10) . . ?
U2 U3 U2 89.879(13) 2_655 . ?
U1 U3 U2 59.500(9) . . ?
U4 U3 U2 60.308(9) . . ?
O1 U4 O1 88.2(2) . 2_655 ?
O1 U4 O2 140.63(15) . 2_655 ?
O1 U4 O2 79.02(15) 2_655 2_655 ?
O1 U4 O2 79.02(15) . . ?
O1 U4 O2 140.63(15) 2_655 . ?
O2 U4 O2 132.1(2) 2_655 . ?
O1 U4 O5 138.34(15) . 2_655 ?
O1 U4 O5 79.70(15) 2_655 2_655 ?
O2 U4 O5 75.94(17) 2_655 2_655 ?
O2 U4 O5 85.52(17) . 2_655 ?
O1 U4 O5 79.70(15) . . ?
O1 U4 O5 138.34(15) 2_655 . ?
O2 U4 O5 85.52(17) 2_655 . ?
O2 U4 O5 75.93(17) . . ?
O5 U4 O5 133.4(2) 2_655 . ?
O1 U4 O13 68.53(14) . 2_655 ?
O1 U4 O13 68.68(14) 2_655 2_655 ?
O2 U4 O13 72.13(15) 2_655 2_655 ?
O2 U4 O13 135.97(15) . 2_655 ?
O5 U4 O13 138.38(15) 2_655 2_655 ?
O5 U4 O13 69.79(15) . 2_655 ?
O1 U4 O13 68.68(14) . . ?
O1 U4 O13 68.53(14) 2_655 . ?
O2 U4 O13 135.97(15) 2_655 . ?
O2 U4 O13 72.14(15) . . ?
O5 U4 O13 69.79(15) 2_655 . ?
O5 U4 O13 138.38(15) . . ?
O13 U4 O13 118.9(2) 2_655 . ?
O1 U4 N2 135.90(11) . . ?
O1 U4 N2 135.90(11) 2_655 . ?
O2 U4 N2 66.06(11) 2_655 . ?
O2 U4 N2 66.06(11) . . ?
O5 U4 N2 66.69(11) 2_655 . ?
O5 U4 N2 66.69(11) . . ?
O13 U4 N2 120.54(10) 2_655 . ?
O13 U4 N2 120.53(10) . . ?
O1 U4 U3 31.60(10) . . ?
O1 U4 U3 80.44(11) 2_655 . ?
O2 U4 U3 158.42(11) 2_655 . ?
O2 U4 U3 69.22(11) . . ?
O5 U4 U3 106.76(11) 2_655 . ?
O5 U4 U3 105.82(11) . . ?
O13 U4 U3 94.25(10) 2_655 . ?
O13 U4 U3 37.42(10) . . ?
N2 U4 U3 135.134(8) . . ?
O1 U4 U3 80.44(11) . 2_655 ?
O1 U4 U3 31.60(10) 2_655 2_655 ?
O2 U4 U3 69.22(11) 2_655 2_655 ?
O2 U4 U3 158.42(11) . 2_655 ?
O5 U4 U3 105.82(11) 2_655 2_655 ?
O5 U4 U3 106.76(11) . 2_655 ?
O13 U4 U3 37.42(10) 2_655 2_655 ?
O13 U4 U3 94.25(10) . 2_655 ?
N2 U4 U3 135.133(9) . 2_655 ?
U3 U4 U3 89.733(17) . 2_655 ?
O1 U4 U2 30.83(10) . . ?
O1 U4 U2 80.43(11) 2_655 . ?
O2 U4 U2 109.85(11) 2_655 . ?
O2 U4 U2 103.86(11) . . ?
O5 U4 U2 157.76(11) 2_655 . ?
O5 U4 U2 68.85(11) . . ?
O13 U4 U2 37.98(10) 2_655 . ?
O13 U4 U2 93.62(10) . . ?
N2 U4 U2 135.534(8) . . ?
U3 U4 U2 59.883(12) . . ?
U3 U4 U2 59.346(11) 2_655 . ?
C4 O9 U3 141.6(5) . . ?
C1 O8 U3 143.4(5) . . ?
U1 O7 U2 102.35(15) . . ?
U1 O7 U3 102.88(15) . . ?
U2 O7 U3 102.58(16) . . ?
C5 O6 U3 132.1(4) . . ?
C8 O5 U4 138.6(5) . . ?
C2 O4 U3 139.0(5) 5_655 . ?
C6 O3 U2 137.8(5) . . ?
C5 O2 U4 138.6(4) . . ?
U2 O1 U3 118.93(19) . . ?
U2 O1 U4 117.27(18) . . ?
U3 O1 U4 115.88(18) . . ?
C2 O16 U1 134.2(4) . . ?
U3 O15 U1 117.76(18) . . ?
U3 O15 U2 115.71(19) . 2_655 ?
U1 O15 U2 115.58(17) . 2_655 ?
C4 O14 U2 133.1(4) 5_655 . ?
U3 O13 U2 104.16(17) . 2_655 ?
U3 O13 U4 103.18(15) . . ?
U2 O13 U4 102.78(15) 2_655 . ?
C3 O12 U1 134.3(5) . . ?
C8 O11 U2 131.3(4) . . ?
C3 O10 U2 134.6(4) . . ?
C7 N2 C7 116.7(9) 2_655 . ?
C7 N2 U4 121.7(4) 2_655 . ?
C7 N2 U4 121.7(4) . . ?
O2 C5 O6 127.3(6) . . ?
O9 C4 O14 125.8(7) . 5_655 ?
O4 C2 O16 124.8(7) 5_655 . ?
O17 C1 O8 126.0(8) . . ?
O12 C3 O10 127.7(7) . . ?
O5 C8 O11 127.8(7) . . ?
N2 C7 C10 123.6(7) . . ?
O18 C6 O3 125.6(8) . . ?
C9 C10 C7 119.8(8) . . ?
C15 C14 C13 124.2(8) . . ?
C14 C15 N1 120.6(9) . . ?
C15 N1 C11 116.9(9) . . ?
C13 C12 C11 120.1(9) . . ?
C14 C13 C12 118.4(9) . . ?
C10 C9 C10 116.5(10) . 2_655 ?
C12 C11 N1 119.7(8) . . ?

_refine_diff_density_max         1.122
_refine_diff_density_min         -1.368
_refine_diff_density_rms         0.266

_shelxl_version_number           2014-3



